Views:46 Author:Site Editor Publish Time: 2021-06-28 Origin:Site
Nowadays, aluminum die casting products are more and more widely used in industrial production and life. It is understood that the electroplating of aluminum die casting parts is affected by the special properties of aluminum and requires special pre-treatments. These pre-treatments It needs to be adjusted due to different aluminum materials and different parts, and the general process cannot be simply used. The electroplating pretreatment of aluminum alloy die castings includes four important processes: degreasing, acid etching, chemical plating or displacement plating, and pre-plating. The key is electroless plating or displacement plating. Therefore, the tests that are often done are focused on this process.
The four common electroplating methods for aluminum die casting products are as follows:
1. Phosphating of aluminum materials: The effects of accelerators, fluorides, Mn2+, Ni2+, Zn2+, PO4; and Fe2+ on the phosphating process of aluminum materials have been studied in detail by using methods such as SEM, XRD, potential-time curve, and film weight change. influences. Research shows that guanidine nitrate has the characteristics of good water solubility, low dosage and rapid film formation. It is an effective accelerator for aluminum phosphating: fluoride can promote film formation, increase film weight, and refine grain; Mn2+ and Ni2+ can be obvious Refine the grains to make the phosphating film uniform and compact and improve the appearance of the phosphating film; when the Zn2+ concentration is low, the film cannot be formed or the film formation is poor. As the Zn2+ concentration increases, the film weight increases and the O4 content increases the weight of the phosphate film The impact is greater, increase PO4. The content increases the weight of the phosphating film.
2. Alkaline electrolytic polishing process for aluminum: The alkaline polishing solution system was studied, and the effects of corrosion inhibitors, viscosity agents, etc. on the polishing effect were compared, and an alkaline solution with good polishing effects for zinc-aluminum die castings was successfully obtained. System, and for the first time obtained additives that can lower the operating temperature, prolong the service life of the solution, and at the same time improve the polishing effect. The experimental results show that adding appropriate additives to the NaOH solution can produce a good polishing effect. Exploratory experiments also found that after DC constant voltage electrolytic polishing with glucose NaOH solution under certain conditions, the reflectivity of the aluminum surface can reach 90%, but due to the unstable factors in the experiment, further research is needed. The feasibility of using DC pulse electrolytic polishing method to polish aluminum under alkaline conditions is explored. The results show that the pulse electrolytic polishing method can achieve the leveling effect of DC constant voltage electrolytic polishing, but its leveling speed is slow.
3. Environmentally-friendly chemical polishing of aluminum and aluminum alloys: It is determined to develop a new environmentally-friendly chemical polishing technology using phosphoric acid-sulfuric acid as the base fluid. This technology must achieve zero emission of NOx and overcome the quality defects of similar technologies in the past. The key to the new technology is to add some compounds with special effects to the base fluid to replace nitric acid. For this reason, it is first necessary to analyze the three acid chemical polishing process of aluminum, especially the role of nitric acid. The main function of nitric acid in aluminum chemical polishing is to inhibit pitting corrosion and improve polishing brightness. Combined with the chemical polishing test in simple phosphoric acid-sulphuric acid, it is believed that the special substances added to phosphoric acid-sulphuric acid should be able to inhibit pitting corrosion and slow down overall corrosion, and must have a better leveling and brightening effect.
4. Electrochemical surface strengthening treatment of aluminum and its alloys: the process, performance, morphology, composition and structure of aluminum and its alloys in a neutral system by anodic oxidation and deposition to form ceramic-like amorphous composite conversion coatings are preliminarily discussed. The film forming process and mechanism of the layer. Process research results show that in the Na_2WO_4 neutral mixing system, the concentration of film-forming accelerator is controlled to be 2.5-3.0g/l, the concentration of complexing film agent is 1.5-3.0g/l, and the concentration of Na_2WO_4 is 0.5-0.8g/l , The peak current density is 6-12A/dm-2, and weak agitation can obtain a complete, uniform, and good-gloss gray series inorganic non-metallic film. The thickness of the film is 5-10μm, the microhardness is 300-540HV, and the corrosion resistance is excellent. The neutral system has good adaptability to aluminum alloys, and can form a good film on various series of aluminum alloys such as rust-proof aluminum and forged aluminum.